**Acknowledgements**

The authors would like to thank Dennis Cooper, Brian Webster and Shane Maskill for their assistance with the experimental work.

[4] L. M. Kachanov, "The time to failure under creep condition", *Izv. Akad. Nauk., SSSR.*

Application of the Liu and Murakami Damage Model for Creep Crack Growth Predictions in Power Plant Steels

http://dx.doi.org/10.5772/57052

189

[6] Y. Lui and S. Murakami, "Damage localization of conventional creep damage models and proposition of a new model for creep damage analysis", *JSME International Jour‐*

[7] T. H. Hyde, "Creep crack growth in 316 stainless steel at 600°C", *High Temperature*

[8] D. R. Hayhurst and C. J. Morrison, "Development of continuum damage in the creep

[9] G. A. Webster, S. R. Holdsworth, M. S. Loveday, I. J. Perrin, K. Nikbin, H. Purper, R. P. Skelton, and M. W. Spindler, "A code of practice for conducting notched bar creep rupture tests and for interpreting the data", *J. Fatigue and Fatigue of Eng. Materials and*

[10] C. J. Hyde, T. H. Hyde, W. Sun and A. A. Becker, "Damage mechanics based predic‐ tions of creep crack growth in 316 stainless steel", *Engineering Fracture Mechanics*,

[11] T. H. Hyde, M. Saber and W. Sun, "Testing and modelling of creep crack growth in compact tension specimens from a P91 weld at 650°C," *Engng. Frac. Mech*, 2010,

[12] T. H. Hyde and W. Sun, "Determining high temperature properties of weld materi‐ als," *JSME Int. J. of Solids Mechanics & Material Eng, Series A*, 2000, 43(4), 408-414.

rupture of notched bars", *Phil. Trans. R. Soc. Lond. (A)*, 1984, 311, 103-129.

[5] Y. N. Robotnov, "Creep Problems of Structural Members", *North-Holland*, 1969.

*Tekh. Nauk*, 1958, 8, 26-31.

*Technology*, 1988, 6(2), 51-61.

*Struct*, 2004, 24, 319-342.

2010, 77(12), 2385-2402.

77(15), 2946-2957.

*nal*, 1998, 41, 57-65.
